Metals Additive Manufacturing Powder Aging Characterization
Thomas Lovejoy Nick Muetterties
Mechanical Engineering Department California Polytechnic State University
Statement of Disclaimer
ANALYSIS OF POWDER RECYCLING IN SELECTIVE LASER MELTING
LAWRENCE LIVERMORE NATIONAL LABORATORIESStephen Burke
Matt Wraith Stephen Knaus Thomas Pluschkell
ADDERThomas Lovejoy Nick Muetterties David Otsu
Table of Contents
1 INTRODUCTION ... 10
2 BACKGROUND ... 11
3 DESIGN DEVELOPMENT ... 13
3.1 Overall Experimental Development ... 13
All Identified Tests ... 13
Forming Constraints ... 14
Down-Selection ... 14
Testing Considerations... 15
3.2 Part Development ... 15
KlinoCube ... 15
RadioKnob ... 16
Tensile Coupon ... 17
Residual Stress Bridge ... 17
Residual Stress Comb ... 18
Compression Part ... 18
Other Part ... 18
3.3 Build Plate Development ... 18
Build Plate Design Constraints ... 20
3.4 Custom Instrument Development ... 21
Background ... 21
Ideation ... 22
Design Selection ... 24
Proof of Concept ... 24
Addendum – Custom Spreader Instrument ... 25
4 DESCRIPTION OF FINAL DESIGN ... 27
4.1 Powder Properties ... 28
Particle Size Distribution ... 28
Particle Morphology ... 28
Powder Tap Density ... 28
Powder Absorptivity ... 28
Powder Rheology ... 29
Composition ... 29
4.3 Part Properties ... 29
Microstructure ... 29
Hardness ... 30
Tensile Properties ... 30
Internal Porosity ... 30
Residual Thermal Stress ... 30
Surface Morphology... 31
4.4 Build Plate Final Design ... 31
Parts ... 31
Plate Design... 32
Powder Usage Analysis ... 32
4.5 Custom Rheology Instrument Description ... 34
Physical Description ... 34
Operation ... 35
Data Analysis ... 35
4.6 Final Fabrication Procedures ... 36
Labeling and Packaging ... 38
4.7 LLNL Testing Procedures ... 40
MicroXCT-200 Radiography Instrument ... 40
Malvern Morphologi G3 Instrument ... 40
Absorptivity Instrument ... 40
XPS Analysis ... 41
4.8 PROJECT MANAGEMENT PLAN ... 41
Thomas Lovejoy ... 41
Nicholas Muetterties ... 41
David Otsu ... 42
5 EXPERIMENTAL RESULTS AND DISCUSSION ... 43
5.1 Particle Size Distribution and Morphology ... 43
Beckman Coulter LS230 ... 43
Malvern Morphologi G3 ... 46
Beckman and Malvern Instrumentation Comparison ... 50
Scanning Electron Microscopy ... 53
Beckman Coulter LS230 Particle Size Analyzer ... 55
Scanning Electron Microscopy ... 55
5.3 Tapped Density ... 58
5.4 Powder Absorptivity ... 59
Custom LLNL Powder Absorptivity Instrument ... 59
5.5 Compositional Analysis ... 61
X-Ray Fluorescence ... 61
X-ray photoelectron spectroscopy ... 62
5.6 Part Density ... 64
Archimedes’ Density... 64
CT Scan ... 64
5.7 Surface Morphology ... 69
Scanning Electron Microscopy ... 69
5.8 Mechanical Properties ... 73
Rockwell Hardness Tester ... 73
Instron Hydraulic Loadframe ... 78
Tensile Bar Fracture Surfaces ... 81
5.9 Residual Stresses ... 88
5.10 Custom Angle of Repose Instrument ... 89
As Constructed Design ... 89
Calibration ... 90
Results ... 90
5.11 Addendum – Microstructural Analysis ... 91
Kalling’s Etch ... 91
Electrolytic Oxalic Etch ... 92
5.12 Powder Spreader Proof of Concept ... 93
6 CONCLUSIONS ... 95
6.1 Recommendations ... 95
Powder Sampling Techniques ... 95
Oversized Powder Analysis ... 95
Copper Composition Changes Induced by Wire EDM ... 95
Compositional Trends ... 95
Quantifiable Surface Morphology Measurements ... 96
Table of Figures
Figure 1. Schematic of SLM process. ... 10
Figure 2. Isometric view of the KlinoCube. ... 16
Figure 3. Modification of KlinoCube extrusion. ... 16
Figure 4. Isometric view of RadioKnob. ... 16
Figure 5. Isometric view of Tensile Coupon. ... 17
Figure 6. Isometric view of Residual Stress Bridge. ... 17
Figure 7. Isometric view of Residual Stress Comb. ... 18
Figure 8. MLab powder volume with respect to cycles. ... 19
Figure 9. MLab powder height with respect to cycles. ... 20
Figure 10. Angle of repose concept image... 25
Figure 11. Powder spreader instrument conceptual design. a) Static lighting element for consistent shadow formation. b) Powder tray. c) Powder laid flat by spreading apparatus. d) Spreading apparatus. ... 26
Figure 12. Example particle morphologies. ... 28
Figure 13. Commercial purity molybdenum microstructure. ... 30
Figure 14. Example surface morphology. ... 31
Figure 15. Height of build chamber powder vs cycles. ... 33
Figure 16. Solidworks model of custom rheology isntrument. ... 34
Figure 17. Example angle analysis. ... 36
Figure 18. Beckman Coulter LS230 particle size distribution for normal run powder across cycles. The distribution for all runs appears nearly identical with only slight variation in the mean size or distribution shape. ... 44
Figure 19. Mean particle diameter equivalent for cycles 1-9. ... 45
Figure 20. Standard Deviation for cycles 1-9. ... 45
Figure 21. Malvern Morphologi G3 particle size distribution by number %. ... 47
Figure 22. Malvern Morphologi G3 circularity distribution by number %. ... 48
Figure 23. Malvern Morphologi G3 convexity distribution by number %. ... 48
Figure 24. Run 1 particle size distribution comparison. ... 50
Figure 25. Run 3 particle size distribution comparison. ... 51
Figure 26. Run 5 particle size distribution comparison. ... 51
Figure 27. Run 7 particle size distribution comparison. ... 52
Figure 28. Run 9 particle size distribution comparison. ... 52
Figure 30. Representative SEM image from CP Run 9 powder sample... 54
Figure 31. Beckman Coulter particle size distribution of oversized powder samples 1-9. The distribution starts as bimodal with the separation occurring around 50 microns then over cycles becomes more unimodal. ... 55
Figure 32. Clusters and large particles from Oversized Run 9 powder sample. ... 56
Figure 33. Clusters, large particles, and super particle from Oversized Run 9 powder sample. ... 57
Figure 34. Tested and Bulk density for powder over cycles. ... 58
Figure 35. Run 1 powder absorptivity measurements. ... 59
Figure 36. Run 5 powder absorptivity measurements. ... 60
Figure 37. Run 9 powder absorptivity measurements. ... 60
Figure 38. Calculated Archimedes' Density results for KlinoCubes 2-10 ... 64
Figure 39. MATLAB visualization of of CT scan video for Run 5. ... 65
Figure 40. Porosity vs. frame for Run 1. ... 65
Figure 41. Porosity vs. frame for Run 5. ... 66
Figure 42. Porosity vs. frame for Run 10.. ... 66
Figure 43. Modified internal porosity visualization for Run 5. ... 67
Figure 44. LLNL and MATLAB internal porosity visualization. ... 68
Figure 45. Surface morphology of Run1 KlinoCube side with XY plane angled 45° above scale-bar line. ... 70
Figure 46. Surface morphology of Run 4 KlinoCube with XY plane perpendicular to scale-bar line. 70 Figure 47. Surface morphology of Run 10 KlinoCube with XY plane perpendicular to scale-bar line. ... 71
Figure 48. Cracks seen in Run 2 KlinoCube with XY plane parallel to scale-bar line. ... 71
Figure 49. Surface morphology of top surface of Run 4 KlinoCube. Removed extrusion depicted in lower-left corner of image. ... 72
Figure 50. Close up surface morphology of top surface near semi-circle extrusion of Run 4 KlinoCube. ... 72
Figure 51. Tensile bar face numbers. ... 73
Figure 52. Ultimate strength in ksi over cycles. ... 79
Figure 53. Elastic Modulus of the tensile specimens over cycles ... 79
Figure 54. Percent elongation at fail for tensile specimens over cycles. ... 80
Figure 55. Propgating cracks on the side of tensile specimen 2A. ... 80
Figure 56. Overlay of stress-strain curves for annealed tensile specimens 1A, 5A, and 10A. ... 81
8 Figure 58. Reverse fracture surface from Run 1 as-fabricated tensile bar. Red arrow denotes print
direction. a) Patterned circular pores. ... 84
Figure 59. Fracture surface from Run 10 as-fabricated tensile bar. a) Large cone-shaped pore. b) Slit-like pores. ... 85
Figure 60. Reverse fracture surface of Run 10 as-fabricated tensile bar. a) Location of skin-effect (Figure 42)... 86
Figure 61. Skin-effect seen in the as-fabricated Run 10 tensile bar fracture surface. ... 87
Figure 62. Angle of deflection for each bridge. ... 88
Figure 63. Angle of Repose results from the custom built instrument. ... 90
Figure 64. Cycle 10 Square extrusion. Large pore with incoherent spherical particle. Waterless Kalling's. ... 92
Figure 65. 200x magnification of the square extrusion from the Run 1 KlinoCube. ... 92
Figure 66. 100x magnifiication of the triangle extrusion from the Run 1 KlinoCube. Depicted are incompletely coalesced weld layers predicted to result in the slit-like pores seen in the tensile bar fracture surfaces. ... 93
Figure 67. Components used for powder spreader instrument. ... 94
List of Tables
Table I. Accepted angle of repose values of common materials. ... 23
Table II. Summary of properties and analysis methods ... 27
Table III. Individual Part Volumes ... 31
Table IV. Powder Volume Consumed per Cycle ... 32
Table V. Powder Remaining per Cycle ... 32
Table VI. Scale of powder flowability based on angle of repose. ... 36
Table VII. Malvern Morphologi G3 Statistics ... 46
Table VIII. XRF compositions from run powder samples ... 61
Table IX. XRF compositions from oversized powder samples ... 61
Table X. XRF compositions from KlinoCubes ... 62
Table XI. XPS surface compositions from run powder samples ... 62
Table XII. XPS surface compositions from RadioKnobs ... 63
Table XIII. Approximate Percent Porosity for Runs 1, 5, and 10. ... 67
Table XIV. Tensile specimen dimensions and results ... 78
Table XV. Mechanical properties with and without the inclusion of specimens 1A, 2A, 4A and 7A. .. 78
Table XVI. Angle of deflection for each run. ... 88
Selective laser melting (SLM) is an Additive Manufacturing (AM) process in which a bed of metallic powder is melted with a guided laser to form a solid piece of metal. Layers of powder are deposited and melted on top of each other to produce a 3D part (Figure 1). This promising new technology enables the fabrication of complex part geometries previously unattainable through conventional manufacturing processes .
Despite the potential of SLM, there are still many technical challenges that must be overcome. The recycling characteristics of powder are one of the challenges that have not been sufficiently addressed. In SLM, a blade is used to spread a fresh layer of powder on top of the previous consolidated layer. An inconsistent powder bed will inevitably result in manufacturing defects, such as poor surface finish, warpage, excessive porosity, and undesirable
mechanical properties. In order to have homogeneous and dense layers, SLM requires highly spherical, normally distributed powder sizes in the range of 10-50 microns with sufficient flowability. Unfortunately, this cannot be guaranteed in practice. Because it is cost
prohibitive to use fresh new powder for every single build, it is standard practice to sieve, recycle, and reuse the powder left over from the previous build. However, the powder properties can change unpredictably over the course of many cycles . Another source of variation is in the powder manufacturing process itself. These methods yield variations in powder size, morphology, and composition unique to each one. Consequently, it is essential to have well defined specifications when ordering powder from manufacturers. The current knowledge base is insufficient for
generating such comprehensive specifications. A final source of powder variation is the effects of oxygen and moisture. It has been demonstrated from preliminary studies that oxygen absorption is possibly one of the key factors influencing mechanical properties .
Despite the importance of powder characteristics, research in this area is in the nascent stage. Some of the preliminary work has been summarized in literature . Among these efforts is a study on AM metal powder characterization using an extensive array of techniques applied to both virgin and recycled powder states . However, this report focuses solely on the powders; the link between the powder characteristics and the manufactured part properties, which is essential to AM industry, is not addressed. Moreover, whether these techniques are sufficient and necessary to characterize powder properties for AM is still unclear. Other studies fail to address the effects of post-fabrication powder sieving and losses to HEPA filtration, further complicating the
interpretation of the results .
11 The multidisciplinary undergraduate engineering team at Cal Poly SLO (CP) is working together with Lawrence Livermore National Lab (LLNL) to address these issues and develop SLM
technologies. The year-long research project has three primary objectives:
1. Discover how metallic powder evolves across build cycles and time,
2. Verify the relationships between metallic powder attributes and final part properties, and 3. Develop new instruments and novel characterization techniques.
The work being done in this project builds off of a lot of previous work. While additive manufacturing (AM) is still budding technology, many parameters have already been studied extensively. The work most relevant to this project is that related to the powder used and how it ages with reuse.
Once a part is finished, common practice in AM is to recycle the unused powder for the next build. However, due to partial sintering and melting effects, the recycled powder’s properties deviate from the original. At present time there is little conclusive data or standardization on the full effects of powder aging.
In late 2014, the National Institute of Standards and Technology (NIST) released a comprehensive literature review of work related to manufacturing entitled Measurement Science Needs for Real-time Control of Additive Manufacturing Powder Bed Fusion Processes. It provides summaries of numerous studies while also presenting any correlations found between process parameters and part qualities. The breadth of the studies presented is substantial, and is broken up by pre-process, in-process, and post-process measurements. Many of these studies, including those from Ning et al, Wang, Wegner and Witt, found that the in-process variables that most affect the final part are scan speed, laser power, scan spacing, and layer thickness. These are exclusively in-process
measurements, and thus outside the scope of the experiment .
The main focus of the NIST review was on AM parts with little consideration of how aged powder affects them. Some of the most critical conclusions are mentioned below. The most common parameters mentioned within the scope of the project are the powder density and particle size distribution.
Spierings et al. found that a threshold relative powder density is required for the production of fully dense parts. From this it was concluded that powder grain size distribution and density are critical variables in consistent mechanical properties. The Archimedes method was also confirmed to have low uncertainty and great repeatability  . Research from Gu et al. also pointed out the
importance of the powder morphology, with spherical powder repeatedly outperforming irregular-shaped powder in mechanical properties .
12 Weingarten et al. studied various drying methods in Formation and reduction of hydrogen porosity during selective laser melting of AlSi10Mg. It was found that 96% of gas content in part voids was hydrogen. The concentration of hydrogen comes from the moisture present on the powder and in the machine prior to building. Drying the powder before use can reduce hydrogen content upwards of 50% .
Kempen et al studied hardness, microstructure, as well as scan speed in Microstructure and mechanical properties of SLM 18Ni-300 Steel. Their experimentation concluded that an increase in scan speed or layer thickness results in a decrease in macrohardness and relative density. It was also found that the density deficit can be recovered by re-melting the metal i.e. scanning the whole part twice .
Given the spectrum of parameters that effect part builds, it’s difficult to obtain a comprehensive description of a powder’s characteristics from one test as Clayton et al points out in The Application of Powder Rheology in Additive Manufacturing. As a result they performed four different tests. First, it was found that reduced permeability and increased specific energy are correlated to poor layer uniformity, which leads to imperfections in the final part. The second study compared “identical” powders from two different suppliers and found a fair amount of variation in powder properties. The third study found that small quantities of additives in powder blends can have a significant effect on the permeability and flowability of feedstock. The fourth part of the study examined the flow differences between virgin powder, recycled powder, and a blend of the two. It was found that the flowability of blends does not change linearly with respect to virgin powder added .
In Characterization and Control of Powder Properties Strondl et al discuss the flow properties of new and used powders. It was found that recycled SLM powders have a better flowability than new powders, possibly due to the decrease in finer particles. It was also found that porosity in final parts is higher when made from recycled powders. These parts also have lower ductility and impact toughness. The parameters studied that have the largest influence on mechanical properties were oxygen content and porosity .
The following section outlines the development of the overall experiment. A necessary subset of this was the design of parts for comprehensive characterization of post-fabrication properties. Once this was completed, the focus was shifted to the actual build plates to be fabricated by LLNL’s machines. Additionally, a need was identified for a custom rheology instrument – the steps taken to develop this instrument are outlined in this section as well.
Overall Experimental Development
The development of the overall experiment began with a literature review to identify all material properties relevant to this project for both pre-processed powder and post-fabricated parts. Once a list of properties was constructed, the team formed constraints to aid in down-selection. These constraints were applied to the list of properties, resulting in a final list of 11 properties. The characterization methods corresponding to each property was identified and arrangements were made to conduct analysis for the project.
All Identified Tests
After an extensive literature search, the following powder properties were identified as those which could potentially change over the course of build cycles and have an effect on the final fabricated parts:
Powder PropertiesParticle Size Distribution
Particle Morphology Thermal Conductivity Absorptivity Tap Density Rheology Composition
Additionally, the following part properties were identified as those which would be affected by any changes induced by the recycling of the feed powder:
Part PropertiesComposition Fatigue Strength Tensile Properties Compressive Properties Microstructure Hardness Porosity Fracture Strength
The following constraints were formed in order to systematically eliminate less-valuable tests from the focus of this project:
With the maximum testing period estimated to be 10 weeks, all properties and cycles must be able to be analyzed within this timeframe.
All properties should be selected with the goal of minimizing cost to this project. If the analysis must be performed at CP, the combined service fees must amount to $100 per cycle or below. If the analysis must be performed by LLNL, approval is subject to the sponsor’s discretion. Any test that must be performed by a contractor outside of CP and LLNL must not exceed the price of $50.00 per specimen. If equipment must be purchased and exceeds $500 in value, there must be a justifiable reason outside of this project to purchase.
126.96.36.199 Part Geometry
All part properties requiring specimens larger than the build volumes provided cannot be selected. Properties requiring specimens with extensive post-processing are undesirable.
Safety - Any test that would require training in excess of 1 month, safety equipment exceeding $200.00 in value, or poses extreme risk of danger or loss of life to the operator is considered extremely undesirable.
With these constraints in mind, the following tests were eliminated from the focus of this project: 188.8.131.52 Fatigue Strength
Fatigue strength analysis can require many weeks to perform. Justifying reservations of the necessary testing equipment would be difficult. For these reasons, fatigue strength was removed from the scope of this project.
184.108.40.206 Fracture Strength
Fracture strength analysis requires specimens of precisely controlled dimensions. Aside of the extensive post-processing required for each specimen, the test itself can be subject to low robustness. For these reasons, fracture strength was removed from the scope of this project. 220.127.116.11 Compressive Properties
For metals, compression properties derived from a uniaxial compression test are relatively similar to tension analysis. Additionally, compression specimens are subject to more safety concerns during testing. For these reasons, compressive properties were removed from the scope of this project.
18.104.22.168 Overhang Analysis
Overhang analysis was considered extensive enough to be its own individual senior project. For this reason, it was removed from the scope of this project.
22.214.171.124 Thermal Conductivity
15 members, it was determined that any custom thermal conductivity instrument would have
intrinsically high variability, potentially invalidating all analysis. For this reason, thermal conductivity was removed from the scope of this project.
With the final properties in mind, the ADDER team at CP established points of contact within the ME, MATE, and DSCI departments to use their instruments for analysis. Additionally, coordination was made between several LLNL facilities for characterization methods unavailable at CP. The final list of properties and their associated tests is outlined in Section 4. When developing the test procedures, the following factors were accounted for:
126.96.36.199 Time Constraints
Some of the analysis methods require excessive time to perform. Properties that require more than 90 minutes per cycle to analyze are considered a roadblock to the completion of this project. For this reason, these properties will be analyzed on the first, middle, and last cycles only. If there is sufficient evidence that the properties have changed significantly between these three cycles, additional tests will be authorized and conducted.
188.8.131.52 Nuisance Factors
Attempts were made to identify all nuisance factors in order to reduce their effect on the response variables of interest. The following factors were identified:
Humidity - As a known and uncontrollable factor, humidity will be monitored during all stages of powder handling and analysis. Analysis of covariance will be carried out if its assumptions are met over the course of the experiment. Additionally, all powder samples shall be kept in desiccated storage environments.
Order of Treatments - It is unknown how the order of analysis will affect the responses. To combat this, all tests shall be carried out in a random order to reduce the potential effects of this nuisance factor.
In order to effectively test a wide variety of properties several parts were needed – often with a part being used for multiple tests. Through discussion with LLNL the importance of certain properties were deemed of lesser or higher importance in part design and selection. Drawings for each part can be found in Appendix B.
The KlinoCube, shown in Figure 2, was previously designed by LLNL and features three extrusions each with different cross-sectional geometries – a semicircle, a square, and a triangle. The
16 Figure 2. Isometric view of the KlinoCube.
In the conceptual phase, the extrusions were manipulated via solid modeling to include twists, notches, and other cross-sectional geometries. One of these iterations is shown in Figure 3. The original scaled-down model was ultimately chosen as many of the modifications detracted from the part’s manufacturability and relevance to metallographic examination. Additional
Figure 3. Modification of KlinoCube extrusion.
The RadioKnob, depicted in Figure 4, shall be used by LLNL for radiographic porosity analysis. Its geometry has been designed to conform to the requirements of the instrument’s operators. Since porosity is a high priority property and the RadioKnob is very small, it was selected for both the MLab and M2 build series.
One part that was deemed a necessity was a tensile coupon. For the MLab build plate the “sub-size” rectangular tensile design, shown in Figure 5, shall be printed and tested as per ASTM standard E8. The selections of “sub-size” and rectangular cross-section were to conserve volume use. Prior to tensile testing, the grip ends of the tensile bar will be used for testing hardness.
Figure 5. Isometric view of Tensile Coupon.
Since the M2 build volume is much larger, volume constraints will be less pressing. Consequently the tensile coupon used for the M2 build series can be larger and of a different cross section.
Residual Stress Bridge
The Residual Bridge, shown in Figure 6, shall be used to qualitatively measure the residual thermal stresses developed in the SLM process. These stresses are the result of uneven thermal cycling during the build and are often substantial enough to result in macroscopic deformations.
Figure 6. Isometric view of Residual Stress Bridge.
Residual Stress Comb
Another part that was designed for the detection of residual thermal stresses is the Residual Stress Comb, shown in Figure 7. The comb features a series of thin legs – with three sets differing in diameter. When sectioned off, the deflection of each leg and the connecting portion would be observed.
Figure 7. Isometric view of Residual Stress Comb.
For the MLab build series, the comb was not selected as it would likely be redundant with the results from the Residual Bridge. However, the Comb may be used for the M2 build to see if any of the additional variables affect the development of residual thermal stresses.
In the conceptual phase, the development of a compression part was discussed but ultimately abandoned. A lattice structure, often used for compression purposes, is common in many LLNL designs and was mentioned as a structure worth exploring. However performing compression tests presented many safety concerns and would likely produce data that was redundant with the tensile test. Additionally the properties affecting the integrity of the lattice intricacy would be captured in other tests. Consequently, a compression part was never fully designed.
Also discussed in the conceptual phase was the development of an “Other Part” to primarily test tolerances. It was never deemed a high priority, as most properties affecting tight tolerances and intricacies will be observed in other tests.
Depending on the feedback from the MLab build series, an “Other Part” could be added to the M2 build series.
Build Plate Development
19 powder or parts can be observed. These two considerations in conjunction drive a need to balance the number of parts per cycle and number of cycles.
Compounded with the volume constraint was a height constraint – because the entire build volume must be filled to the height of the tallest part. Subsequently, a Microsoft Excel program was created in order to model powder losses through successive cycles. The program takes into account the total build volume for the particular machine, and allows the user to select which parts, how many parts, and the amount of powder to be taken for a build plate. Based on suggestions made, the program also allows a pattern of 3 different plates to be modelled in order to limit the amount of powder lost each cycle while still allowing for the different tests to be performed. The powder volume remaining is graphed as well as powder bed height. Figure 8 and Figure 9 show the results from the program. The red line in Figure 9 shows the height of the tallest part, the KlinoCube. Since building must cease when the amount of powder remaining is no longer able to construct an entire part, the maximum expected cycles for the MLab is 10 cycles.
20 Figure 9. MLab powder height with respect to cycles.
Build Plate Design Constraints
Additionally, to help guide the layout design of each build plate the following quantitative requirements were outlined.
184.108.40.206 Minimizing Height
Minimizing height was deemed important due to space limitations that arise once powder bed levels become low. Parts will not complete fabrication if the height of the powder in the bed becomes less than the height of the part. With this in mind and considering that all build plates should be as similar as possible, it was decided to minimize the height of the parts across all build plates.
220.127.116.11 Minimize Part Contact with Plate
In order to minimize residual thermal stresses while maximizing exposed surface area of the parts, it was decided to minimize the contact area of parts with the plate. This requirement has been made based on recommendations by the machine operators.
18.104.22.168 Maximize Space Between Parts/Even Distribution
Maximizing space between parts reduces unintentional thermal interactions. In comparison with building in a small subsection of the plate, spreading the parts out results in a uniform and
distributed heat affected zone. In doing so, this would also increase the amount of powder affected by the laser. This is important, as small areas of unused powder heavily affected by the laser would be difficult to representatively sample.
22.214.171.124 Uniformity across Different Build Plates
21 126.96.36.199 Safety Margin of 20%
It was observed that up to 20% of powder volume is lost due to HEPA filtering and metal vaporization. Thus, a safety margin of at least 20% powder volume was identified based on feedback given by the machine operators.
Custom Instrument Development
In order to characterize powder with regards to flowability, a custom instrument needed to be investigated in order to fit with existing testing criteria. The process for creating the instrument is outlined below followed by a description of the final design.
In Selective Laser Melting applications, powder flowability presents an ever present concern when considering moving powder from feed hoppers to build volume. In addition, it is crucial that the distribution of particles on the top layer of powder remain as consistent as possible across the build area as new layers are applied. Currently, there are few studies that have explored power rheology with respect to metal powders as used in SLM. Those that have referenced flowability fail to relate the property to other powder characteristics.
Granular materials such as metal powders exhibit properties of all three states of matter and therefore behave unlike any other materials. The understanding of powders is very poor although in recent years, the number of studies focusing on granular flow have increased over tenfold, as new technologies have demanded further understanding of these complex substances .
However, most of these studies originate in the pharmaceutical industry. One comprehensive study done by G. Lumay, et al. states that granular materials experience complex transitions between static and dynamic states and that the motion of the grains is influenced by (i) the steric repulsions, (ii) the friction forces, and (iii) the cohesive forces . Furthermore:
“The steric repulsion is related to the geometry of the grains. The friction forces are influenced by the surface properties and by the chemical nature of the grains. Finally, the cohesive forces are induced by the presence of liquid bridges, electric charges, van der Waals interactions and magnetic dipole– dipole interactions. The granular materials can be split in two categories: cohesive and non-cohesive
granular materials. In non-cohesive granular materials, the interaction between the grains is mainly related to the steric repulsion and to the friction forces. Therefore, the macroscopic properties of the assembly are governed by the geometry of the grains (shape and size distribution) and by the surface properties of the grains. When the cohesive forces between the grains become greater than the weight of one grain, the macroscopic properties are strongly influenced by the cohesion inside the packing. Therefore, when the grains become smaller, the macroscopic properties of the assembly are mainly governed by the cohesive forces.”
22 There exist several testing methods that aim to provide an understanding to the ability of a
granular material to flow. Most, if not all of these methods, have been developed by the food or drug industry, particularly the pharmaceuticals industry. Standard methods include angle of repose and other handling angles, standardized flow rate, apparent and tapped density, and shear cells.
With the exception of shear cells, these methods have demonstrated the dependence on particle shape and distribution as well as temperature and humidity to its ability to flow . Shear cells on the other hand provide insight into the intrinsic nature of the frictional and cohesive forces
between the particles by applying a known load to a bed of powder and measuring the shear forces generated by the powder. As Guerin et al. points out, the shear cell methodology consumes time and product and furthermore, “all these approaches present a major disadvantage being that they are too product consuming, particularly during the first step of a novel drug development when only a very little amount of the product is available” . Herein lies the issue of many of these methods with regards to characterizing the flow properties of metal powders – they consume too much powder. It was thus determined to use a novel testing method for flowability
characterization of powder.
In addition, many other professional laboratory instruments were investigated, though ultimately, each test proved again to either consume a large amount of powder and time or cost well above what a senior project should cost, especially when looking at 11 other properties during the study.
In order to fit with the general testing criteria, the design criteria for the custom instrument includes the following:
• Limit the powder sample • Short time to run each test • Ease of use/modularity
Limiting the powder sample used by the machine was selected as a major design criteria due to the lack of powder available during testing, particularly when sampling from the MLab SLM machine. Based on powder usage analysis in Section 3.3, the maximum amount of powder available for testing each cycle while still maintaining about 9-10 samples was about 1 cubic inch. As a factor of safety against random losses, the maximum amount of powder to be used by the machine had to be below 1 cubic inch and our goal design uses only 0.5 cubic inches.
Furthermore, based on the number of tests run during this experiment and the limitations of time for the lifespan of the project, time to run each sample was also selected as a major design
consideration. As many of the existing methods of powder flow characterizations are time dependent, this device needed to be as time independent as possible to allow for rapid testing of samples. In addition, the device would need to be used to quickly characterize powder in a
manufacturing setting. Arbitrarily, the maximum time to run a sample, including setup, testing, and cleanup was made to be less than 15 minutes.
23 any existing solutions or infrastructure in a facility and increase its ability to be adapted to any situation.
Angle of repose has proven to be a good indicator of flowability and many known standards exist for several materials. Table I below shows these known standards. In addition, it is the simplest of tests to perform and only requires the powder to flow and settle under its own weight. Existing angle of repose methods could be scaled down to fit with stated design criteria. Standardized flowrate would also be easy to perform, but variability/uncertainty in the results would likely lead to poor data from such a test, particularly with the amount of powder available.
Shear cells would give more insightful data about the powder, however, no machines exist that fit the design requirements.
Table I. Accepted angle of repose values of common materials.
Material Angle of Repose (degrees)
Asphalt (crushed) 30–45° Bark (wood refuse) 45°
Clay (dry lump) 25–40° Clay (wet excavated) 15°
Clover seed 28°
Coconut (shredded) 45° Coffee bean (fresh) 35–45°
Flour (corn) 30–40°
Flour (wheat) 45°
Gravel (loose dry) 30–45° Gravel (natural w/ sand) 25–30°
Sand (dry) 34°
Sand (water filled) 15–30°
Sand (wet) 45°
Urea (Granular) 27°
After consideration of the design criteria, a novel method of testing angle of repose was selected as the best solution for the given challenge. This method will consist of quickly raising a vertical tube filled with powder and allowing the powder to flow under its own weight and settle into a conical shape. The angle of repose could then be measured using an image captured by any camera and analyzed with any image processing software. Since the ImageJ software is already in use during this experiment, it will also be used for this method. Additionally, many smartphone cameras have the capability to take high quality photos which will be sufficient for this application.
This method was selected based on the small amount of powder required for each sample and the repeatability of results. A similar test was considered using a scaled down version of a fixed funnel method which could consume similar amounts of powder. However, the powder would need to be manually fed into such a machine which could alter the repeatability of the test. To maintain the integrity of testing conditions for the final design, a high speed linear actuator will be used to raise the glass tube, ensuring a consistent and repeatable motion. Results can then be compared with known values of other powders in order to determine the quality of flowability of the powder.
Proof of Concept
In order to ensure the feasibility of the design, a proof of concept test was run. The test involved using two different tube sizes and manually lifting the tube for several common household powders with known angles of repose. The materials used are listed below.
• Black ceramic tile • White ceramic tile
• 3/8” I.D. copper pipe coupling
• 5/8” I.D. plastic sprinkler extension pipe Powders
• Powdered sugar • Cornstarch • Granulated sugar • Flour
25 Figure 10. Angle of repose concept image. Powder is granulated sugar dispensed from a copper coupling.
The image was then run through ImageJ image processing software, calling upon a function
designed to give an angle between two vectors. Several trials were run for the same conditions and the angles of repose measured and averaged to give a final angle for the material. Results showed that the individual tests varied between about 15° and 29° for the white sugar, with the mean and standard deviation at 24° and 3° respectively. Concerns were raised about the magnitude of the variance between tests, however this proof of concept did not address many uncontrolled variables, particularly the characteristics of the lifting of the tube. According to Zhichao Liu in Measuring the Angle of Repose of Granular Systems Using Hollow Cylinders the method of raising the tube has an effect on the resulting angle of repose . The final prototype will be built to address these
variables. Additionally, the average angle of repose measured was less than the known value of 37°. Again, this variance could be due to errors in the testing variables, however, for the final design, a thorough calibration will be done in order to account for any further differences encountered.
The proof of concept test resulted in important conclusions to be addressed in final prototype design. The first being control of test variables, particularly the lifting characteristics. Secondly, camera placement and angle can skew the angle seen in the captured image. Standards for these variables will need to be developed in order to further minimize variance in determined angles. Furthermore several runs are required for each sample in order to form a statistical profile of the sample.
Addendum – Custom Spreader Instrument
26 Figure 11. Powder spreader instrument conceptual design. a) Static lighting element for consistent shadow formation. b)
DESCRIPTION OF FINAL DESIGN
The following properties are the focus of this senior project, shown in Table II. The standard operating procedures for all properties analyzed by Cal Poly are outlined in Appendix A. The desired analysis and results for all properties analyzed by LLNL are outlined in Section 4.7.
Table II. Summary of properties and analysis methods
Property Analysis Method Operator Cycles to Analyze
Particle Size Distribution Coulter LS220 PSA CP
Malvern G3 Morphologi LLNL
Particle Morphology Malvern G3 Morphologi
First, Middle, Last
Powder Tapped Density Vibes Table Adapter
Powder Absorptivity Custom Absorptivity Instrument
First, Middle, Last
Powder Angle of Repose Angle of Repose Instrument
Powder Spread Quality Spreader Instrument
General Composition X-Ray Fluorescence
Surface Composition X-Ray Photoelectron Spectroscopy
First, Middle, Last
First, Middle, Last
Instron Hydraulic Loadframe
First, Middle, Last
Residual Thermal Stresses
Particle Size Distribution
Particle size distribution (PSD) is a record of particle sizes in a sample of powder. During the melting process, many of the particles nearby are partially sintered together, resulting in
conglomerate particles in the recycled powder. This was found to raise the average particle size as much as 37% . Many of the smaller particles are also lost to the in-process ventilation and recycling. The combination of increasing particle size and loss of smaller particles creates more gaps between powder particles, resulting in a decreased tap density and increased part porosity. PSD shall be analyzed with the Beckman Coulter LS230 PSA.
The morphology of a particle is classified by ASTM B243. In general, the processes used to fabricate metallic AM powders produce nearly spherical particles with few defects. As the powder added to the AM machine undergoes build cycles, irregular shapes become more common due to
agglomeration and partial sintering effects (Figure 12). These irregular shapes may result in a reduction of packing efficiency, resulting in larger individual pores in the part and subsequent deterioration of mechanical properties . Morphology shall be characterized by LLNL using their Malvern G3 Morphologi instrument. As a second measure, CP will also characterize particle morphology under the SEM.
Figure 12. Example particle morphologies. Particles imaged with a SEM.
Powder Tap Density
The apparent density of the powder when it is allowed to settle under its own weight is called the tap density. This is an important in-process property, as inefficiently packed powder may result in increased porosity. It is expected that the tap density will decrease due to an increase in particle size variation. Additionally, non-spherical particles may also decrease the tap density of the overall powder . Tap density shall be analyzed by CP with the DSCI Tap Density instrument.
29 absorptivity will decrease. Absorptivity shall be analyzed with LLNL custom absorptivity
Rheology refers to the study of the flow of a material. Quantitatively, rheology can be expressed by several different parameters, such as deformation, stress, viscosity, and coefficient of friction. Powder rheology has been selected because of its importance in SLM applications. How the powder flows influences the manner in which it fed into the build volume. Previous studies have shown that flow properties may be related to particle size distribution, particle morphology, and other powder properties. However, these connections have not been explored within additive manufacturing applications. Based on previous studies, it is expected that flowability of the powder will increase with subsequent cycles, resulting in a decrease in angle of repose. Rheology shall be characterized with the Custom Rheology Instrument, found in Section 4.5.
Powder and Part Properties
The relative amounts of each element in an alloy plays an important role in the material’s
mechanical and physical properties. It is possible that the SLM process selectively vaporizes certain elements at its high operating temperatures. Additionally, segregated elemental distribution may occur during heating and cooling of the unused powder . Over many cycles, these compositional gradients may result in unfavorable changes to the properties of the fabricated parts. Because of this, composition is an important property to monitor during the SLM process. Composition shall be characterized with x-ray fluorescence and x-ray photoelectron spectroscopy.
Microstructure refers to the microscale grain structure of the material. It provides information about past processing conditions such as cooling rates, heat treatments, thermal gradients, and strain directions. The morphology of the phases, the degree of porosity, and the presence of inclusions aids one in predicting the structural behavior of the material. Analyzing the
30 Figure 13. Commercial purity molybdenum microstructure.
Hardness is a measurement of the mechanical properties on the surface of a sample. Because it is a quick and relatively simple characterization method, it stand as an efficient way of validating the mechanical properties of the specimen. Hardness with be characterized with a Rockwell Hardness Tester.
The tensile properties of a material serve as representative mechanical values when designing for load bearing applications. The most common and important properties are elastic modulus, yield strength, ultimate tensile strength, and percent elongation. These values are heavily affected by the geometry and microstructure of the final part. Inclusions, porosity, surface finish, and grain
structure all affect tensile properties in different ways. Previous studies have shown conflicting powder recycling results, potentially due to differences in material systems  . It is the goal of this project to look at the tensile properties of the fabricated parts in conjunction with other
material attributes in order to make meaningful connections between both groups. Tensile properties shall be analyzed by CP with an Instron Hydraulic Loadframe.
Internal porosity is the result of trapped gases, incomplete melting, and inefficient packing during the SLM process. Previous modelling attempts have shown that non-uniform size distribution allows smaller spherical particles to fill the space between larger spheres, increasing the packing efficiency and reducing the overall porosity of the fabricated parts . As the powder undergoes cycles in the machine, the distribution and particle morphology may change, resulting in an increase or decrease in porosity. Porosity shall be analyzed by LLNL with their MicroXCT200 instrument. Additionally, it will also be measured indirectly by CP through Archimedes’ principle.
Residual Thermal Stress
31 with respect to recycled powder, it has been selected as an important property to monitor. Residual stresses shall be visually documented by CP and modelled using finite element analysis.
The surface morphology of the fabricated part has a large effect on its mechanical properties. Irregularities can act as stress concentrators, resulting in strength values much lower than
expected. Parts fabricated by SLM have surface morphologies largely dependent on the particle size distribution, particle morphologies, and orientation in the machine . Depending on how these properties change, the surface morphology could be affected as well. The surface morphology of parts shall be analyzed by CP through SEM imaging.
Figure 14. Example surface morphology. Depicted are partially sintered particles on the surface of a part.
Build Plate Final Design
Exactly 2 Tensile Bars, 1 KlinoCube, 1 RadioKnob, and 1 Bridge shall be incorporated into the build plate design. In total, the 5 parts will consume 1.0605 in3 of powder per cycle (Table III). Drawings
for each part can be found in the Appendix at the end of this report.
Table III. Individual Part Volumes
Part Name Number Volume/Cycle (in3)
Tensile Bar 2 0.6
KlinoCube 1 0.318
RadioKnob 1 0.005
Bridge 1 0.1375
The build plate shall be designed according to the following criteria:
• Minimize potential interaction between parts through even spacing
• Minimize build height in order to maximize the total amount of powder available for fabrication
• Interface the parts with the surface of the build plate in such a way that minimizes the number of processes necessary to retrieve the parts in shipping condition
An example build plate is provided in the Appendix at the end of this report to demonstrate all parts fit while meeting the aforementioned design criteria.
Powder Usage Analysis
Each cycle is predicted to require approximately 3.06 in3 of powder: 1.06 in3 for building parts, 1.5
in3 for powder samples, and a nominal safety margin of 0.5 in3 to account for standard operational
losses. Assuming a total of 39.4 in3 of powder (equivalent to the entire MLab build volume) is
initially utilized for this experiment, the MLab machine shall complete 8 build cycles (Table IV and Table V). The limiting factor is the height of the tallest part on the plate – once the remaining volume of powder is unable to fill the chamber to this height, it must cease operation (Figure 15). (The tallest part, KlinoCube, is estimated to be 0.975 in tall when placed on the build plate
according to the designer’s recommendations.)
Table IV. Powder Volume Consumed per Cycle Component Volume/Cycle (in3)
All Parts 1.0605
CP Powder Sample 1
LLNL Powder Sample 0.5
Safety Margin 0.5
Table V. Powder Remaining per Cycle
Number Remaining (inPowder 3) in Chamber (in) Powder Height
0 39.40 3.138
1 36.33 2.894
2 33.27 2.650
3 30.21 2.406
4 27.15 2.163
5 24.09 1.919
6 21.03 1.675
7 17.97 1.431
8 14.91 1.188
33 Figure 15. Height of build chamber powder vs cycles.
Custom Rheology Instrument Description
The final instrument design for the custom rheology test is outlined in the following sections. Operating procedures and additional materials are also found below.
The custom rheology instrument to be developed will be composed of the materials shown in Table C1 in Appendix C. In addition, a rendering of the instrument assembly can be found in Figure 16. The main support for the structure is a heavy duty lab stand with a platform and column upon which other parts are attached. Starting from the bottom up, the powder platform consists of a collection dish and a platform upon which the powder will be released. The
collection dish exists to collect the superfluous powder in the sample that falls off of the platform above. The platform is approximately 0.5 inches in diameter which will form a cone with a maximum volume of 0.03 cubic inches for an angle of repose of 60° which is beyond the expected range of values for the measured angle of repose. In addition, 0.03 cubic inches is significantly smaller than the design criteria specifies, however, when adding superfluous powder to ensure a full cone on the platform, the total powder added to the machine will likely total to approximately 0.1 cubic inch – again below the specified criteria. The entire piece will likely be constructed from 3D printed extruded ABS plastic. However, the top surface of the platform is covered by a paper disc cut to the
aforementioned size. This material is used in other rheology applications and according to the study done
by Liu, surface roughness has an effect on the resulting angle of repose seen . Therefore, this and other materials will be tested during calibration of the machine to see which material gives the best result.
Above the platform, the glass borosilicate tube rests, guided by one or two plastic bushings held by clamps. The bushings will ensure that the tube only moves in the vertical direction and eliminate any unwanted movement during operation. The glass tube has an inner diameter of approximately 0.315 inches (8mm) and will be cut to a length of about 3 inches. The diameter of the tube was selected to be smaller than the diameter of the platform in order to ensure a seal between the two to limit any powder leaking from the tube skewing results. Gracing the top of the glass tube is the coupler to attach the tube to the linear actuator. This piece will also be constructed of 3D printed ABS plastic and will feature a funnel shape in the interior to aid in pouring powder into the tube. Connecting the coupling to the tube will be accomplished using a polyurethane adhesive.
A high speed linear actuator is used to lift the tube off of the platform. The decision to use a linear actuator for this application resulted from the need to produce a repeatable and consistent tube lifting profile. Furthermore, this particular actuator, the specification sheet of which can be found
35 in Appendix D, strokes at a rate of 9 inches per second. Compared to other actuators of this size, this was the highest speed available. Rational thought brings one to believe that a slow lifting speed will influence the way the powder flows out from the bottom of the tube, possibly slowing the powder or forcing the powder to flow radially outward rather than down. Therefore, to remove these undesirable effects the tube would ideally just disappear, however, a rapid upward
movement is the only practical solution. In this way, the powder will be allowed to flow under its own weight, uninterrupted by obstacles. Powering the linear actuator is a 12V DC power supply. A polarity reversing switch is used to extend and retract the actuator stroke.
Basic operation of the device consists of setting the position of the actuator based on platform and tube height, adding a sample to the tube, connecting the tube and actuator, and finally retracting the stroke. Each time the machine is run, the height of actuator needs to be set in order to ensure a tight seal between the bottom of the tube and the platform. To accomplish this, hold the tube tightly on the platform, then extend the stroke of the actuator fully. Place the end of the stroke into the coupler on top of the tube. Insert the coupling pin to ensure a proper fit, then remove it. Tighten the two clamps holding the actuator to the stand to secure the actuator. The stroke can then be detracted to allow powder to be poured into the tube. A detailed procedure can be found in the Custom Rheology Instrument SOP in Appendix A.
Data reporting shall follow procedures outlined in the Custom Rheology Instrument SOP in
Appendix A. Data outputs of the device will include 3 images from each sample. Each image will be processed separately by an image processing software. For this experiment, ImageJ will be used to determine the angle of repose. This process consists of:
1) Opening ImageJ software
2) Opening the desired image in the program 3) Selecting the ‘Angle’ tool from the ImageJ toolbar
4) Clicking on a point on one side of the pile along the horizontal (at the base of the cone) 5) Clicking again on the point on the other side of the pile where the angle meets the base of
the cone. A line should be drawn between the two points, ideally this line is perfectly horizontal.
6) Moving the mouse over to the top of the cone at the top point. A line should be connected from point in step 5 to the cursor location. Ensure the cursor (or line) is located/passes through exactly at the top point of the pile. The line does not have to be contained within the pile or stay out of the outline of the pile, as long as the two points for the line are at the bottom corner and top corner. DO NOT CLICK AT THIS POINT.
7) Recording the angle given by ImageJ. In the ImageJ toolbar, several values are shown including x and y locations as well as angle.
36 Figure 17. Example angle analysis. ImageJ software utilized to measure the angle.
Correlations between the value of angle of repose and other properties measured will be explored. In addition, the values will be compared to other materials with known values in order to
determine the “flowability” of the powder based on the scale shown in Table VI below.
Table VI. Scale of powder flowability based on angle of repose.
. Flow Property Angle of Repose (°) Hausner ratio
Excellent 25-30 1.00-1.11
Good 31-35 1.12-1.18
Fair 36-40 1.19-1.25
Passable 41-45 1.26-1.34
Poor 46-55 1.35-1.45
Very poor 56-65 1.46-1.59
Very very poor ≥66 ≥1.60
Final Fabrication Procedures
37 188.8.131.52 Concept Laser MLab Fabrication Procedures
A. Before powder is added to the machine, take 6 samples of powder from the source of virgin powder. These samples are to serve as controls unaffected by the SLM process. Each sample shall be approximately 2 in3 (33 mL) and shall be placed in the appropriate
container sized by LLNL and labeled according to the labeling procedures listed in Section 184.108.40.206. Desired powder sampling procedures based off ASTM B215 are described as follows:
a. Ensure powder is thoroughly mixed.
b. Pull 5 individual samples from the powder such that the total volume of the samples equals the total desired sample size. (Individual = 0.4 in3, Total = 2 in3) Vary the
location from which the individual samples are taken in all 3 directions in order to achieve a representative total sample of the entire powder volume.
Specific measuring techniques will be left to the operator’s discretion,
keeping in mind: contamination, losses of smaller particles due to air/motion, and exposure to the environment.
B. Fill the entire Concept Laser MLab hopper with virgin powder.
C. Initialize the Concept Laser MLab with the build plate design, similar to the one depicted in section 4.4.2.
D. Begin filling out the Log Sheet provided at the end of this report.
• This sheet is used to track ambient and operating variables. A new Log Sheet shall be filled out anytime the machine is run.
E. Run the Concept Laser MLab machine to build the parts.
• All of the powder shall be put through to the build volume. The exact procedure for this is left to the discretion of the operator, and could be accomplished by running the powder through the applicator layer by layer, speeding up the rate of application after parts are finished, or manually dumping the remaining feed lot powder into the build space.
F. Brush all of the powder into the overflow container and clean the build plate appropriately. At this point, all of the powder shall be in the overflow container and ready to be sieved. G. Sieve the powder with a 50 micron filter.
• Powder removed during sieving shall be stored for future analysis
• If necessary, further mix the powder after sieving to ensure a homogeneous state. H. If this is an odd numbered cycle, take a powder sample of 1.0 in3 for Cal Poly and another
sample of 0.3 in3 for LLNL.
• The 1.0 in3 sample will be placed in an appropriately sized container, labeled
according to the labeling procedures listed in Section 220.127.116.11, and shipped to Cal Poly.
• The 0.3 in3 sample will be placed in an appropriately sized container, labeled
according to the labeling procedures listed in Section 18.104.22.168, and kept at LLNL for testing in the G3 Morphologi and absorptivity instruments.
• Following this procedure will result in powder sampling on every other cycle I. Place the remaining powder back into the feed lot to be run again.
38 K. Exactly one tensile bar, selected at random, shall be heat treated according to LLNL’s
standard heat treatment procedures for Nitronic 40 parts • No other parts shall undergo heat treatment
L. Label and package fabricated parts according to the labeling procedure outlined in Section 22.214.171.124.
M. Repeat steps C-K until any of the following conditions are met: 1) 10 cycles are reached, 2) the level of powder remaining does not allow for the completion of an entire build cycle, 3) particle size/powder quality diminishes to a point that the machine becomes inoperable 4) operator’s discretion.
The log sheet included with this report shall be used to track operating variables and provide space for in-process observations to be recorded. The second half of the page is the space for those observations to be written down with guiding section titles on the left. It is highly recommended that notes are made about each cycle, particularly with regards to:
• Any issues that arise during fabrication.
• Issues that arise during sampling (both parts and powder).
• The quality of the parts being produced and any defects (to compare with parts received). • The amount of powder and other material that gets sieved out of the powder lot (is there a
particular point at which an unusual amount of powder starts to get sieved out?).
Labeling and Packaging
Powder samples will all be labeled according to the following properties: A. Material
B. Cycle C. Date
D. Approximate Volume
A sticker sheet template is included in the Appendix at the end of this report which includes all of the above properties and can serve as a guide or can be used in conjunction with the appropriate sticker sheet in order to print labels. This method is suggested as all labels will be consistent and will be easiest for the operator to fill out. The labels should be completed in pen and initialed by the operator.
The sticker sheet template is compatible with the following Avery Products:
15162, 15662, 18162, 18662, 48462, 48862, 5162, 5262, 5662, 5962, 8162, 8252, 8462, 8662, 88662, 95662, 18262
39 126.96.36.199 Parts
The 2 tensile bars, 1 KlinoCube, and 1 Bridge are for Cal Poly characterization. The 1 RadioKnob is for LLNL characterization. The Cal Poly parts shall be placed in a clear, re-sealable plastic bag (like a Ziploc bag). The LLNL part shall be placed in a separate clear, re-sealable plastic bag. Therefore, there shall be two bags per build plate that together contain all of the parts. Both bags shall be sealed with as much of the air inside pushed out, so as to limit the chances of the bag popping during handling.
Each bag shall be labeled with the following information: A. Material
B. Cycle C. Date 188.8.131.52 Shipping
Samples will be shipped as seen fit by LLNL to Cal Poly. All efforts shall be made to ensure that samples are not damaged or contaminated in any way during transit. The shipping address for all shipments is:
Mustang ’60 Machine Shop Cal Poly
1 Grand Ave.
LLNL Testing Procedures
MicroXCT-200 Radiography Instrument
The MicroXCT-200 Radiography machine shall be used to characterize the RadioKnob part for its density and internal porosity. In total, three RadioKnobs will be characterized: the first cycle, the last cycle, and the median cycle. The observations to be made are as follows:
• The percentage of the overall part volume that is occupied by air/pores (% by volume porosity)
• One .AVI video file of the part scanned longitudinally (square cross-sections) • One .AVI video file of the part scanned transversely (circle cross-sections)
All information from this instrument should be labelled appropriately with regards to the build cycle that the part came from. The video files should contain information about the scale of the part with respect to the pixels displayed (for example, microns per frame slice and microns per pixel). In total, 2 video files and 1 porosity reading shall be recorded for each part and submitted to Cal Poly for additional analysis.
All used and un-used RadioKnobs shall be kept for the duration of this experiment in the event that more data is required.
Malvern Morphologi G3 Instrument
The Malvern Morphologi G3 instrument shall be used to characterize the LLNL powder samples for particle size and morphology. Based on operator estimates, approximately 0.1 in3 of the 0.3 in3
powder sample designated for LLNL shall be used for each observation. In total, powder samples from four cycles shall be characterized. The cycles selected shall vary based on how many are completed. However, the first and last cycle powder samples shall be characterized no matter what. The other two cycles shall be evenly spaced between the cycles. The observations to be made in order of importance are as follows:
• Aspect ratio (shape) • Circular equivalent (size) • Circularity (shape) • Convexity (shape) • Solidity (shape)
All information from this instrument should be labelled appropriately with regards to the build cycle that the powder sample came from.
All used and un-used powder samples shall be kept for the duration of this experiment in the event that more data is required.
The custom absorptivity instrument shall be used to characterize the LLNL powder samples for absorptivity measurements. Based on operator estimates, approximately 0.1 in3 of the 0.3 in3